Structural and Magnetic Characteristics of Gd5GaxSi4-x
Hui Wang; Sumohan Misra; Fei Wang; Gordon J. Miller; Inorganic Chemistry 49 (2010) 4586–4593; doi:10.1021/ic100142u

data_4315499
_publ_section_title
;
 Structural and Magnetic Characteristics of Gd5GaxSi4-x
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4586
_journal_page_last               4593
_journal_paper_doi               10.1021/ic100142u
_journal_volume                  49
_journal_year                    2010
_chemical_formula_sum            'Ga0.63 Gd5 Si3.38'
_chemical_formula_weight         924.63
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.4845(10)
_cell_length_b                   14.833(2)
_cell_length_c                   7.8087(11)
_cell_measurement_reflns_used    6985
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      28.26
_cell_measurement_theta_min      2.75
_cell_volume                     866.9(2)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0428
_diffrn_reflns_av_sigmaI/netI    0.0294
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            6985
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         28.26
_diffrn_reflns_theta_min         2.75
_exptl_absorpt_coefficient_mu    39.990
_exptl_absorpt_correction_T_max  0.2781
_exptl_absorpt_correction_T_min  0.134
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS; Sheldrick 2003'
_exptl_crystal_colour            metallic
_exptl_crystal_density_diffrn    7.084
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1547
_exptl_crystal_size_max          0.05026
_exptl_crystal_size_mid          0.041
_exptl_crystal_size_min          0.032
_refine_diff_density_max         2.258
_refine_diff_density_min         -1.272
_refine_diff_density_rms         0.335
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     49
_refine_ls_number_reflns         1083
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.078
_refine_ls_R_factor_all          0.0283
_refine_ls_R_factor_gt           0.0233
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0222P)^2^+0.7225P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0491
_refine_ls_wR_factor_ref         0.0507
_reflns_number_gt                964
_reflns_number_total             1083
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic100142u_si_001_1.cif
_cod_data_source_block           Gd5Ga0.63Si3.37
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4315499